Loading in 5 sec....

Electronic Structure of Rocksalt Copper Monoxide: A Proxy for High Temperature SuperconductivityPowerPoint Presentation

Electronic Structure of Rocksalt Copper Monoxide: A Proxy for High Temperature Superconductivity

- 104 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about ' Electronic Structure of Rocksalt Copper Monoxide: A Proxy for High Temperature Superconductivity' - amaranta-nova

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

Electronic Structure of Rocksalt Copper Monoxide: A Proxy for High Temperature Superconductivity

Paul M. GrantIBM Research Staff Member, Emerituswww.w2agz.com

Journal of Physics: Conference Series 129 (2008) 012042

http://www.iop.org/EJ/article/1742-6596/129/1/012042/jpconf8_129_012042.pdf

Abstract. Cubic rocksalt copper monoxide, in contrast to its lighter transition metal neighbours, does not exist in nature nor has it yet been successfully synthesized. Nonetheless, its numerical study as a structurally simpler proxy for the layered cuprate perovskites may prove useful in probing the source of high temperature superconductivity in the latter family of compounds. We report plane-wave pseudopotential DFT (LDA+U) results for both cubic and tetragonal CuO and find rather surprisingly a metallic band structure persists for 0 < U < 6 eV, and c/a = 1 with a Mott-Hubbard gap opening only for finite U under a tetragonal distortion, e.g., above c/a = 1.1 for U = 6. The metallic states display a Fermi surface with clear nesting tendencies suggesting that high temperature superconductivity in copper oxide compounds may be at least initially mediated by Jahn-Teller electron-phonon coupling as originally proposed by Bednorz and Mueller.

“Should be Metals, But Aren’t” (Charge Transfer Insulators, Instead)

After Imada, et al, RMP 70, 1039 (1998)

Cubic Rocksalt Divalent TMOs

TMO 3d Config Properties

MnO 5 MH-CTI (5.6)

FeO 6 MH-CTI (5.9)

CoO 7 MH-CTI (6.3)

NiO 8 MH-CTI (6.5)

CuO 9

XX Doesn't Exist!

See Imada, Fujimore, Tokura, RPM 70 (1988)

Experimental Equipment (Software)

QUANTUM-ESPRESSO Suit of Codes

DFT (LDA+U) plus electron-phonon

Graphics by Tone Kolalj (XCrysDen)

www.quantum-espresso.org

“Dial-in” Parameters

G2 = 40 Ry ρ = 320 Ry

Convergence ≤ 10-6 Ry

“Smearing” = Methfessel-Paxton

Psuedopotentials: Ultrasoft, XC = Perdew-ZungerCu: 3d94s2 O: 2s22p4

c-rs-CuO Basic Asymmetric AF Cell

c/a = 1.36

Measurements(Wolter Siemons)

- 2-4 ML epi on STO
- No Fermi Edge
- No Exchange Bias on ferro-SRO (Tc ~ 100-150 K)

5.320

3.905

3.905

Cubic

Tetragonal

Spin Composition of Cu 3d pDOS as fn(Hubbard): c/a = 1.36

U = 0 d-spin-pdos Cu1

U = 5 d-spin-pdos Cu1

W. Siemons (PhD Thesis, Stanford)

EF

t-CuO Density-of-States

N(E) (eV-1)

E (eV)

Non-Magnetic Cubic Rocksalt CuO-- Electron-Phonon Properties --

λ ~ 0.6 – 0.7

Other sc’s…

α2F(ω)

k << EF

σ = 0.04

Conclusions & Homework

Conclusions

c-rs-CuO is metallic and thus a proxy for HTSC cuprates.

e-p λ ~ 0.6 – 0.7 consistent with TC ~ 20 – 50 K.

t-rs-CuO becomes a MH-CTI for c/a >~ 1.1, U > 3 eV.

c/a < 1.1, t-rs-CuO is “self-doped” metal.

DFT (LDA+U) + proxy structures a useful exploratory tool for nano-material discovery.

Homework

Compute e-p coupling λ as f(c/a,U) for t-rs-CuO.

Compute TN, µ*, BCS prefactor, then TC .

Compute isotope shift.

Calculate optical & transport properties as f(c/a).

Investigate larger values of a-lattice constant

Download Presentation

Connecting to Server..